Presentation on theme: "Characteristics of Metals Important in Sheet Forming"— Presentation transcript:
1Characteristics of Metals Important in Sheet Forming Metal Forming CourseCharacteristics of Metals Important in Sheet Forming
2Localized Necking in Sheet Metal Metal Forming CourseLocalized Necking in Sheet Metal(a) Localized necking in a sheet specimen under tension. (b) Determination of the angle of neck from the Mohr’s circle for strain. (c) Schematic illustration for diffuse and localized necking. (d) Localized necking in an aluminum strip stretched in tension. Note the double neck.
3Yield Point Elongation Metal Forming CourseYield Point Elongation(a) Yield point elongation and Lueder’s bands in tension testing. (b) Lueder’s bands in annealed low-carbon steel sheet. (c) Stretcher strains at the bottom of a steel can for household products.
4Metal Forming Course Shearing Schematic illustration of the shearing process with a punch and die. This process is a common method of producing various openings in sheet metals.
5Characteristics of Hole and Slug Metal Forming CourseCharacteristics of Hole and SlugCharacteristic features of (a) a punched hole and (b) the punched slug. Note that the slug has been sealed down as compared with the hole.
6Metal Forming Course Shearing (a) Effect of clearance c between the punch and die on the deformation zone in shearing. As clearance increases, the material tends to be pulled into the die, rather than being sheared. In practice, clearances usually range between 2% and 10% of the thickness of the sheet. (b) Microhardness (HV) contours for a 6.4-mm-thick AISI 1020 hot-rolled steel in the sheared region.Typical punch-penetration curve in shearing. The area under the curve is the work done in shearing. The shape of the curve depends on process parameters and material properties.
7Punching, Blanking and Shearing Operations Metal Forming CoursePunching, Blanking and Shearing OperationsPunching (piercing) and blanking. (b) Examples of various shearing operations on sheet metal.
8Metal Forming Course Fine Blanking (a) Comparison of sheared edges by conventional (left) and fine-blanking (right) techniques. (b) Schematic illustration of the setup for fine blanking.
9Metal Forming Course Bending (a) Bending terminology. The bend radius is measured to the inner surface of the bend. Note that the length of the bend is the width of the sheet. Also note that the bend angle and the bend radius (sharpness of the bend) are two different variables. (b) Relationship between the ratio of bend radius to sheet thickness and tensile reduction of area for various materials. Note that sheet metal with a reduction of area of about 50% can be bent and flattened over itself without cracking.
10The Effect of Elongated Inclusions Metal Forming CourseThe Effect of Elongated Inclusions(a) and (b) The effect of elongated inclusions on cracking as a function of the direction of bending with respect to the original rolling direction. This example shows the importance of the direction of cutting from large sheets in workpieces that are subsequently bent to make a product. (c) Cracks on the outer radius of an aluminum strip bent to 90˚.
11Metal Forming Course Springback in Bending Terminology for springback in bending. It is caused by the elastic recovery of the material upon unloading. In this example, the material tends to recover toward its originally flat shape. However, there are situations where the material bends further upon unloading (negative springback).
12Metal Forming Course Negative Springback Schematic illustration of the stages in bending round wire in a V-die. This type of bending can lead to negative springback, which does not occur in free bending.
13Methods of Reducing or Eliminating Springback Metal Forming CourseMethods of Reducing or Eliminating SpringbackMethods of reducing or eliminating springback in bending operations.
14Common Die-Bending Operations Metal Forming CourseCommon Die-Bending OperationsCommon die-bending operations, showing the die-opening dimension W used in calculating bending forces.
15Metal Forming Course Roll-Forming Process The roll-forming process. Stages in roll forming of a sheet-metal door frame. In Stage 6, the rolls may be shaped as in A or B.
16Metal Forming Course Tube Forming A method of forming a tube with sharp angles, using axial compressive forces. Compressive stresses are beneficial in forming operations because they delay fracture. Note that the tube is supported internally with rubber or fluid to avoid collapsing during forming.
17Stretch-Forming Process Metal Forming CourseStretch-Forming ProcessSchematic illustration of a stretch-forming process. Aluminum skins for aircraft can be made by this process.
18Bulging Of A Tubular Part Metal Forming CourseBulging Of A Tubular Part(a) Bulging of a tubular part with a flexible plug. Water pitchers can be made by this method. (b) Production of fittings for plumbing by expanding tubular blanks with internal pressure. The bottom of the piece is then punched out to produce a “T.” (c) Manufacturing of Bellows.
19Metal Forming Course Hydroform Process The hydroform, or fluid-forming, process. Note that, unlike in the ordinary deep-drawing process, the dome pressure forces the cup walls against the punch. The cup travels with the punch, and thus deep drawability is improved.
20Tube-Hydroforming Process Metal Forming CourseTube-Hydroforming Process(a) Schematic illustration of the tube-hydroforming process. (b) Example of tube-hydroformed parts. Automotive exhaust and structural components, bicycle frames, and hydraulic and pneumatic fittings are produced through tube hydroforming.
21Metal Forming Course Spinning Processes Schematic illustration of spinning processes: (a) conventional spinning and (b) shear spinning. Note that in shear spinning, the diameter of the spun part, unlike in conventional spinning, is the same as that of the blank. The quantity f is the feed in mm/rev.
22Explosive Forming Process Metal Forming CourseExplosive Forming ProcessSchematic illustration of the explosive-forming process. Although explosives are generally used for destructive purposes, their energy can be controlled and employed in forming large parts that would otherwise be difficult or expensive to produce by other methods.
23Metal Forming Course Deep-drawing Process (a) Schematic illustration of the deep-drawing process. The stripper ring facilitates the removal of the formed cup from the punch. (b) Variables in deep drawing of a cylindrical cup. Only the punch force in this illustration is a dependent variable; all others are independent variables, including the blankholder force.
24Deformation in Flange and Wall in Deep Drawing Metal Forming CourseDeformation in Flange and Wall in Deep DrawingDeformation of elements in (a) the flange and (b) the cup wall in deep drawing of a cylindrical cup.
25Metal Forming Course Draw Bead (a) Schematic illustration of a draw bead. (b) Metal flow during drawing of a box-shaped part, using beads to control the movement of the material. (c) Deformation of circular grids in drawing.
26Metal Forming Course Ironing Process Normal Anisotropy Schematic illustration of the ironing process. The cup wall is thinner than its bottom. All beverage cans without seams (known as two-piece cans) are ironed, generally in three steps, after being deep drawn into a cup. (Cans with separate tops and bottoms are known as three-piece cans.)Normal AnisotropyDefinition of the normal anisotropy ratio, R, in terms of width and thickness strains in a tensile-test specimen cut from a rolled sheet. The specimen can be cut in different directions with respect to the length, or rolling direction, of the sheet.
27Average Normal Anisotropy Metal Forming CourseAverage Normal AnisotropyTypical range of the average normal anisotropy ratio, R, for various sheet metals.
28Effect of Average Normal Anisotropy Metal Forming CourseEffect of Average Normal AnisotropyEaring in a drawn steel cup, caused by the planar anisotropy of the sheet metal.
29Metal Forming Course Deep Drawing Effect of die and punch corner radii in deep drawing on fracture of a cylindrical cup. (a) Die corner radius too small. The die corner radius should generally be 5 to 10 times the sheet thickness. (b) Punch corner radius too small. Because friction between the cup and the punch aids in the drawing operation, excessive lubrication of the punch is detrimental to drawability.
30Metal Forming Course Redrawing Operations Reducing the diameter of drawn cups by redrawing operations: (a) conventional redrawing and (b) reverse redrawing. Small-diameter deep containers undergo many drawing and redrawing operations.
31Forming-Limit Diagram (FLD) Metal Forming CourseForming-Limit Diagram (FLD)(a) Forming-limit diagram (FLD) for various sheet metals. The major strain is always positive. The region above the curves is the failure zone; hence, the state of strain in forming must be such that it falls below the curve for a particular material; R is the normal anisotropy. (b) Note the definition of positive and negative minor strains. If the area of the deformed circle is larger than the area of the original circle, the sheet is thinner than the original, because the volume remains constant during plastic deformation.